#------------------------------------------------------------------------------
#$Date: 2021-04-16 12:25:10 +0300 (Fri, 16 Apr 2021) $
#$Revision: 264250 $
#$URL: file:///home/coder/svn-repositories/cod/cif/1/56/18/1561866.cif $
#------------------------------------------------------------------------------
#
# This file is available in the Crystallography Open Database (COD),
# http://www.crystallography.net/
#
# All data on this site have been placed in the public domain by the
# contributors.
#
data_1561866
loop_
_publ_author_name
'Ward, Matthew D.'
'Oh, George N.'
'Mesbah, Adel'
'Lee, Minseong'
'Sang Choi, Eun'
'Ibers, James A.'
_publ_section_title
;
 Syntheses and characterization of the cubic uranium chalcogenides
 Rh2U6S15, Cs2Ti2U6Se15, Cs2Cr2U6Se15, and Cs2Ti2U6Te15
;
_journal_name_full               'Journal of Solid State Chemistry'
_journal_page_first              14
_journal_page_last               19
_journal_paper_doi               10.1016/j.jssc.2015.04.005
_journal_volume                  228
_journal_year                    2015
_chemical_formula_sum            'Cs2 Te15 Ti2 U6'
_chemical_formula_weight         3703.80
_space_group_crystal_system      cubic
_space_group_IT_number           229
_space_group_name_Hall           '-I 4 2 3'
_space_group_name_H-M_alt        'I m -3 m'
_atom_sites_solution_hydrogens   .
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            4
_cell_length_a                   15.0130(4)
_cell_length_b                   15.0130(4)
_cell_length_c                   15.0130(4)
_cell_measurement_reflns_used    9040
_cell_measurement_temperature    100(2)
_cell_measurement_theta_max      36.45
_cell_measurement_theta_min      2.71
_cell_volume                     3383.78(16)
_computing_cell_refinement       'Bruker SAINT'
_computing_data_collection       'Bruker APEX2'
_computing_data_reduction        'Bruker SAINT'
_computing_molecular_graphics    'Crystalmaker (Palmer, 2013)'
_computing_publication_material  'SHELXL-2014 (Sheldrick, 2014)'
_computing_structure_refinement  'SHELXL-2014 (Sheldrick, 2014)'
_computing_structure_solution    'SHELXS-2014 (Sheldrick, 2014)'
_diffrn_ambient_temperature      100(2)
_diffrn_measured_fraction_theta_full 0.997
_diffrn_measured_fraction_theta_max 0.999
_diffrn_measurement_device_type  'Bruker APEX-II CCD'
_diffrn_measurement_method       'φ and ω scans'
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.0838
_diffrn_reflns_av_unetI/netI     0.0203
_diffrn_reflns_Laue_measured_fraction_full 0.997
_diffrn_reflns_Laue_measured_fraction_max 0.999
_diffrn_reflns_limit_h_max       24
_diffrn_reflns_limit_h_min       -25
_diffrn_reflns_limit_k_max       25
_diffrn_reflns_limit_k_min       -25
_diffrn_reflns_limit_l_max       24
_diffrn_reflns_limit_l_min       -25
_diffrn_reflns_number            39541
_diffrn_reflns_point_group_measured_fraction_full 0.997
_diffrn_reflns_point_group_measured_fraction_max 0.999
_diffrn_reflns_theta_full        25.242
_diffrn_reflns_theta_max         36.450
_diffrn_reflns_theta_min         2.713
_exptl_absorpt_coefficient_mu    43.842
_exptl_absorpt_correction_T_max  0.0925
_exptl_absorpt_correction_T_min  0.0218
_exptl_absorpt_correction_type   numerical
_exptl_absorpt_process_details   'face indexed, SADABS (Sheldrick, 2008)'
_exptl_crystal_colour            black
_exptl_crystal_density_diffrn    7.270
_exptl_crystal_description       block
_exptl_crystal_F_000             5944
_exptl_crystal_size_max          0.241
_exptl_crystal_size_mid          0.155
_exptl_crystal_size_min          0.137
_refine_diff_density_max         4.704
_refine_diff_density_min         -2.143
_refine_diff_density_rms         0.827
_refine_ls_extinction_coef       0.00070(6)
_refine_ls_extinction_expression Fc^*^=kFc[1+0.001xFc²λ³/sin(2θ)]^-1/4^
_refine_ls_extinction_method     SHELXL
_refine_ls_goodness_of_fit_ref   4.656
_refine_ls_hydrogen_treatment    undef
_refine_ls_matrix_type           full
_refine_ls_number_parameters     23
_refine_ls_number_reflns         853
_refine_ls_number_restraints     1
_refine_ls_restrained_S_all      4.653
_refine_ls_R_factor_all          0.0340
_refine_ls_R_factor_gt           0.0340
_refine_ls_shift/su_max          0.001
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'w=1/[σ²(Fo²)] where P=(1.0000Fo²+0.0000Fc²)'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.0855
_refine_ls_wR_factor_ref         0.0855
_reflns_Friedel_coverage         0.000
_reflns_Friedel_fraction_full    .
_reflns_Friedel_fraction_max     .
_reflns_number_gt                853
_reflns_number_total             853
_reflns_threshold_expression     'I > 2σ(I)'
_cod_data_source_file            Cs2Ti2U6Te15A.cif
_cod_data_source_block           Cs2Ti2U6Te15
_cod_original_cell_volume        3383.8(3)
_cod_database_code               1561866
_shelx_space_group_comment
;
The symmetry employed for this shelxl refinement is uniquely defined
by the following loop, which should always be used as a source of
symmetry information in preference to the above space-group names.
They are only intended as comments.
;
_shelxl_version_number           2014-1
loop_
_space_group_symop_operation_xyz
'x, y, z'
'-x, -y, z'
'-x, y, -z'
'x, -y, -z'
'z, x, y'
'z, -x, -y'
'-z, -x, y'
'-z, x, -y'
'y, z, x'
'-y, z, -x'
'y, -z, -x'
'-y, -z, x'
'y, x, -z'
'-y, -x, -z'
'y, -x, z'
'-y, x, z'
'x, z, -y'
'-x, z, y'
'-x, -z, -y'
'x, -z, y'
'z, y, -x'
'z, -y, x'
'-z, y, x'
'-z, -y, -x'
'x+1/2, y+1/2, z+1/2'
'-x+1/2, -y+1/2, z+1/2'
'-x+1/2, y+1/2, -z+1/2'
'x+1/2, -y+1/2, -z+1/2'
'z+1/2, x+1/2, y+1/2'
'z+1/2, -x+1/2, -y+1/2'
'-z+1/2, -x+1/2, y+1/2'
'-z+1/2, x+1/2, -y+1/2'
'y+1/2, z+1/2, x+1/2'
'-y+1/2, z+1/2, -x+1/2'
'y+1/2, -z+1/2, -x+1/2'
'-y+1/2, -z+1/2, x+1/2'
'y+1/2, x+1/2, -z+1/2'
'-y+1/2, -x+1/2, -z+1/2'
'y+1/2, -x+1/2, z+1/2'
'-y+1/2, x+1/2, z+1/2'
'x+1/2, z+1/2, -y+1/2'
'-x+1/2, z+1/2, y+1/2'
'-x+1/2, -z+1/2, -y+1/2'
'x+1/2, -z+1/2, y+1/2'
'z+1/2, y+1/2, -x+1/2'
'z+1/2, -y+1/2, x+1/2'
'-z+1/2, y+1/2, x+1/2'
'-z+1/2, -y+1/2, -x+1/2'
'-x, -y, -z'
'x, y, -z'
'x, -y, z'
'-x, y, z'
'-z, -x, -y'
'-z, x, y'
'z, x, -y'
'z, -x, y'
'-y, -z, -x'
'y, -z, x'
'-y, z, x'
'y, z, -x'
'-y, -x, z'
'y, x, z'
'-y, x, -z'
'y, -x, -z'
'-x, -z, y'
'x, -z, -y'
'x, z, y'
'-x, z, -y'
'-z, -y, x'
'-z, y, -x'
'z, -y, -x'
'z, y, x'
'-x+1/2, -y+1/2, -z+1/2'
'x+1/2, y+1/2, -z+1/2'
'x+1/2, -y+1/2, z+1/2'
'-x+1/2, y+1/2, z+1/2'
'-z+1/2, -x+1/2, -y+1/2'
'-z+1/2, x+1/2, y+1/2'
'z+1/2, x+1/2, -y+1/2'
'z+1/2, -x+1/2, y+1/2'
'-y+1/2, -z+1/2, -x+1/2'
'y+1/2, -z+1/2, x+1/2'
'-y+1/2, z+1/2, x+1/2'
'y+1/2, z+1/2, -x+1/2'
'-y+1/2, -x+1/2, z+1/2'
'y+1/2, x+1/2, z+1/2'
'-y+1/2, x+1/2, -z+1/2'
'y+1/2, -x+1/2, -z+1/2'
'-x+1/2, -z+1/2, y+1/2'
'x+1/2, -z+1/2, -y+1/2'
'x+1/2, z+1/2, y+1/2'
'-x+1/2, z+1/2, -y+1/2'
'-z+1/2, -y+1/2, x+1/2'
'-z+1/2, y+1/2, -x+1/2'
'z+1/2, -y+1/2, -x+1/2'
'z+1/2, y+1/2, x+1/2'
loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_site_symmetry_order
_atom_site_calc_flag
_atom_site_refinement_flags_posn
_atom_site_refinement_flags_adp
_atom_site_refinement_flags_occupancy
_atom_site_disorder_assembly
_atom_site_disorder_group
U1 U 0.0000 0.29453(2) 0.29453(2) 0.00686(13) Uani 1 4 d S T P . .
Cs1 Cs 0.0000 0.5000 0.5000 0.0089(2) Uani 1 16 d S T P . .
Cs2 Cs 0.1408(4) 0.0000 0.0000 0.0203(11) Uani 0.1666 8 d S T P . .
Te1 Te 0.12663(2) 0.12663(2) 0.31337(3) 0.00759(13) Uani 1 2 d S T P . .
Te2 Te 0.2500 0.0000 0.5000 0.00687(17) Uani 1 8 d S T P . .
Ti1 Ti 0.2500 0.2500 0.2500 0.0087(5) Uani 1 12 d S T P . .
loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
Ti Ti 0.2776 0.4457 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Te Te -0.5308 1.6751 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Cs Cs -0.3680 2.1192 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
U U -9.6767 9.6646 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
Te2 U1 Te2 114.456(10) 9 77
Te2 U1 Te1 75.190(8) 9 59
Te2 U1 Te1 142.755(8) 77 59
Te2 U1 Te1 142.755(8) 9 52
Te2 U1 Te1 75.190(8) 77 52
Te1 U1 Te1 77.419(17) 59 52
Te2 U1 Te1 75.190(8) 9 9
Te2 U1 Te1 142.755(8) 77 9
Te1 U1 Te1 73.704(16) 59 9
Te1 U1 Te1 120.10(2) 52 9
Te2 U1 Te1 142.756(8) 9 .
Te2 U1 Te1 75.190(8) 77 .
Te1 U1 Te1 120.10(2) 59 .
Te1 U1 Te1 73.702(16) 52 .
Te1 U1 Te1 77.420(17) 9 .
Te2 U1 Te1 73.882(6) 9 77
Te2 U1 Te1 73.882(6) 77 77
Te1 U1 Te1 140.434(6) 59 77
Te1 U1 Te1 140.434(6) 52 77
Te1 U1 Te1 74.999(12) 9 77
Te1 U1 Te1 75.000(12) . 77
Te2 U1 Te1 73.883(6) 9 30_455
Te2 U1 Te1 73.883(6) 77 30_455
Te1 U1 Te1 74.999(12) 59 30_455
Te1 U1 Te1 74.999(12) 52 30_455
Te1 U1 Te1 140.434(6) 9 30_455
Te1 U1 Te1 140.433(6) . 30_455
Te1 U1 Te1 118.291(18) 77 30_455
Te2 U1 Cs1 57.228(5) 9 .
Te2 U1 Cs1 57.228(5) 77 .
Te1 U1 Cs1 119.948(10) 59 .
Te1 U1 Cs1 119.948(10) 52 .
Te1 U1 Cs1 119.948(10) 9 .
Te1 U1 Cs1 119.948(10) . .
Te1 U1 Cs1 59.146(9) 77 .
Te1 U1 Cs1 59.146(9) 30_455 .
Te2 Cs1 Te2 180.0 57_566 9
Te2 Cs1 Te2 90.0 57_566 77
Te2 Cs1 Te2 90.0 9 77
Te2 Cs1 Te2 90.0 57_566 29_455
Te2 Cs1 Te2 90.0 9 29_455
Te2 Cs1 Te2 180.0 77 29_455
Te2 Cs1 Te1 60.688(4) 57_566 78
Te2 Cs1 Te1 119.312(4) 9 78
Te2 Cs1 Te1 119.312(4) 77 78
Te2 Cs1 Te1 60.688(4) 29_455 78
Te2 Cs1 Te1 119.312(4) 57_566 30_455
Te2 Cs1 Te1 60.688(4) 9 30_455
Te2 Cs1 Te1 60.688(4) 77 30_455
Te2 Cs1 Te1 119.312(4) 29_455 30_455
Te1 Cs1 Te1 180.0 78 30_455
Te2 Cs1 Te1 60.688(4) 57_566 80_455
Te2 Cs1 Te1 119.312(4) 9 80_455
Te2 Cs1 Te1 60.688(4) 77 80_455
Te2 Cs1 Te1 119.312(4) 29_455 80_455
Te1 Cs1 Te1 121.375(8) 78 80_455
Te1 Cs1 Te1 58.625(8) 30_455 80_455
Te2 Cs1 Te1 119.312(4) 57_566 32
Te2 Cs1 Te1 60.688(4) 9 32
Te2 Cs1 Te1 119.312(4) 77 32
Te2 Cs1 Te1 60.688(4) 29_455 32
Te1 Cs1 Te1 58.625(8) 78 32
Te1 Cs1 Te1 121.375(8) 30_455 32
Te1 Cs1 Te1 180.0 80_455 32
Te2 Cs1 Te1 119.312(4) 57_566 79_455
Te2 Cs1 Te1 60.688(4) 9 79_455
Te2 Cs1 Te1 119.312(4) 77 79_455
Te2 Cs1 Te1 60.688(4) 29_455 79_455
Te1 Cs1 Te1 121.375(8) 78 79_455
Te1 Cs1 Te1 58.625(8) 30_455 79_455
Te1 Cs1 Te1 87.634(13) 80_455 79_455
Te1 Cs1 Te1 92.366(13) 32 79_455
Te2 Cs1 Te1 60.688(4) 57_566 31
Te2 Cs1 Te1 119.312(4) 9 31
Te2 Cs1 Te1 60.688(4) 77 31
Te2 Cs1 Te1 119.312(4) 29_455 31
Te1 Cs1 Te1 58.625(8) 78 31
Te1 Cs1 Te1 121.375(8) 30_455 31
Te1 Cs1 Te1 92.366(13) 80_455 31
Te1 Cs1 Te1 87.634(13) 32 31
Te1 Cs1 Te1 180.0 79_455 31
Te2 Cs1 Te1 60.688(4) 57_566 29_455
Te2 Cs1 Te1 119.312(4) 9 29_455
Te2 Cs1 Te1 119.312(4) 77 29_455
Te2 Cs1 Te1 60.688(4) 29_455 29_455
Te1 Cs1 Te1 92.366(13) 78 29_455
Te1 Cs1 Te1 87.634(13) 30_455 29_455
Te1 Cs1 Te1 58.625(8) 80_455 29_455
Te1 Cs1 Te1 121.375(8) 32 29_455
Te1 Cs1 Te1 58.625(8) 79_455 29_455
Te1 Cs1 Te1 121.375(8) 31 29_455
Te2 Cs1 Te1 119.312(4) 57_566 77
Te2 Cs1 Te1 60.688(4) 9 77
Te2 Cs1 Te1 60.688(4) 77 77
Te2 Cs1 Te1 119.312(4) 29_455 77
Te1 Cs1 Te1 87.634(13) 78 77
Te1 Cs1 Te1 92.366(13) 30_455 77
Te1 Cs1 Te1 121.375(8) 80_455 77
Te1 Cs1 Te1 58.625(8) 32 77
Te1 Cs1 Te1 121.375(8) 79_455 77
Te1 Cs1 Te1 58.625(8) 31 77
Te1 Cs1 Te1 180.0 29_455 77
Cs2 Cs2 Cs2 60.0 57 53
Cs2 Cs2 Cs2 90.0 57 9
Cs2 Cs2 Cs2 60.0 53 9
Cs2 Cs2 Cs2 60.0 57 5
Cs2 Cs2 Cs2 90.0 53 5
Cs2 Cs2 Cs2 60.000(1) 9 5
Cs2 Cs2 Te1 148.285(19) 57 5
Cs2 Cs2 Te1 148.285(19) 53 5
Cs2 Cs2 Te1 97.50(5) 9 5
Cs2 Cs2 Te1 97.50(5) 5 5
Cs2 Cs2 Te1 97.50(5) 57 55
Cs2 Cs2 Te1 148.285(19) 53 55
Cs2 Cs2 Te1 148.285(19) 9 55
Cs2 Cs2 Te1 97.50(5) 5 55
Te1 Cs2 Te1 61.23(7) 5 55
Cs2 Cs2 Te1 148.285(19) 57 56
Cs2 Cs2 Te1 97.50(5) 53 56
Cs2 Cs2 Te1 97.50(5) 9 56
Cs2 Cs2 Te1 148.285(19) 5 56
Te1 Cs2 Te1 61.23(7) 5 56
Te1 Cs2 Te1 92.14(12) 55 56
Cs2 Cs2 Te1 97.50(5) 57 6
Cs2 Cs2 Te1 97.50(5) 53 6
Cs2 Cs2 Te1 148.285(19) 9 6
Cs2 Cs2 Te1 148.285(19) 5 6
Te1 Cs2 Te1 92.14(12) 5 6
Te1 Cs2 Te1 61.23(7) 55 6
Te1 Cs2 Te1 61.23(7) 56 6
Cs2 Cs2 Cs2 45.0 57 49
Cs2 Cs2 Cs2 45.0 53 49
Cs2 Cs2 Cs2 45.0 9 49
Cs2 Cs2 Cs2 45.0 5 49
Te1 Cs2 Cs2 133.93(6) 5 49
Te1 Cs2 Cs2 133.93(6) 55 49
Te1 Cs2 Cs2 133.93(6) 56 49
Te1 Cs2 Cs2 133.93(6) 6 49
Cs2 Cs2 Cs1 135.0 57 25_544
Cs2 Cs2 Cs1 135.0 53 25_544
Cs2 Cs2 Cs1 135.0 9 25_544
Cs2 Cs2 Cs1 135.0 5 25_544
Te1 Cs2 Cs1 46.07(6) 5 25_544
Te1 Cs2 Cs1 46.07(6) 55 25_544
Te1 Cs2 Cs1 46.07(6) 56 25_544
Te1 Cs2 Cs1 46.07(6) 6 25_544
Cs2 Cs2 Cs1 180.0 49 25_544
Ti1 Te1 U1 80.771(8) . .
Ti1 Te1 U1 80.771(8) . 5
U1 Te1 U1 161.062(15) . 5
Ti1 Te1 U1 79.106(12) . 81
U1 Te1 U1 90.326(10) . 81
U1 Te1 U1 90.325(10) 5 81
Ti1 Te1 Cs2 116.11(6) . 9
U1 Te1 Cs2 92.157(14) . 9
U1 Te1 Cs2 92.158(14) 5 9
U1 Te1 Cs2 164.79(6) 81 9
Ti1 Te1 Cs1 153.777(16) . 33_445
U1 Te1 Cs1 99.211(8) . 33_445
U1 Te1 Cs1 99.211(8) 5 33_445
U1 Te1 Cs1 74.671(11) 81 33_445
Cs2 Te1 Cs1 90.12(6) 9 33_445
U1 Te2 U1 92.572(2) 34_545 6_556
U1 Te2 U1 92.572(2) 34_545 5
U1 Te2 U1 155.542(10) 6_556 5
U1 Te2 U1 155.542(10) 34_545 81
U1 Te2 U1 92.572(2) 6_556 81
U1 Te2 U1 92.572(2) 5 81
U1 Te2 Cs1 77.771(5) 34_545 33_445
U1 Te2 Cs1 102.229(5) 6_556 33_445
U1 Te2 Cs1 102.229(5) 5 33_445
U1 Te2 Cs1 77.771(5) 81 33_445
U1 Te2 Cs1 102.229(5) 34_545 5
U1 Te2 Cs1 77.771(5) 6_556 5
U1 Te2 Cs1 77.771(5) 5 5
U1 Te2 Cs1 102.229(5) 81 5
Cs1 Te2 Cs1 180.0 33_445 5
Te1 Ti1 Te1 180.0 81 9
Te1 Ti1 Te1 90.690(14) 81 73
Te1 Ti1 Te1 89.310(13) 9 73
Te1 Ti1 Te1 89.310(13) 81 5
Te1 Ti1 Te1 90.690(13) 9 5
Te1 Ti1 Te1 89.310(13) 73 5
Te1 Ti1 Te1 90.690(13) 81 77
Te1 Ti1 Te1 89.310(13) 9 77
Te1 Ti1 Te1 90.690(13) 73 77
Te1 Ti1 Te1 180.0 5 77
Te1 Ti1 Te1 89.310(13) 81 .
Te1 Ti1 Te1 90.690(14) 9 .
Te1 Ti1 Te1 180.0 73 .
Te1 Ti1 Te1 90.690(13) 5 .
Te1 Ti1 Te1 89.310(14) 77 .
loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
U1 Te2 3.1563(2) 9
U1 Te2 3.1563(2) 77
U1 Te1 3.1698(2) 59
U1 Te1 3.1698(2) 52
U1 Te1 3.1698(2) 9
U1 Te1 3.1699(2) .
U1 Te1 3.2639(5) 77
U1 Te1 3.2639(5) 30_455
U1 Cs1 4.3625(4) .
Cs1 Te2 3.75325(11) 57_566
Cs1 Te2 3.75325(10) 9
Cs1 Te2 3.75325(10) 77
Cs1 Te2 3.75325(11) 29_455
Cs1 Te1 3.8832(5) 78
Cs1 Te1 3.8832(5) 30_455
Cs1 Te1 3.8832(5) 80_455
Cs1 Te1 3.8832(5) 32
Cs1 Te1 3.8832(4) 79_455
Cs1 Te1 3.8832(5) 31
Cs1 Te1 3.8832(5) 29_455
Cs1 Te1 3.8832(4) 77
Cs2 Cs2 2.990(8) 57
Cs2 Cs2 2.990(8) 53
Cs2 Cs2 2.990(8) 9
Cs2 Cs2 2.990(8) 5
Cs2 Te1 3.733(4) 5
Cs2 Te1 3.733(4) 55
Cs2 Te1 3.733(4) 56
Cs2 Te1 3.733(4) 6
Cs2 Cs2 4.229(11) 49
Cs2 Cs1 5.392(5) 25_544
Te1 Ti1 2.7868(4) .
Te1 U1 3.1699(2) 5
Te1 U1 3.2639(5) 81
Te1 Cs2 3.733(4) 9
Te1 Cs1 3.8832(4) 33_445
Te2 U1 3.1563(2) 34_545
Te2 U1 3.1563(2) 6_556
Te2 U1 3.1563(2) 5
Te2 U1 3.1563(2) 81
Te2 Cs1 3.75325(10) 33_445
Te2 Cs1 3.75325(10) 5
Ti1 Te1 2.7867(4) 81
Ti1 Te1 2.7867(4) 9
Ti1 Te1 2.7867(4) 73
Ti1 Te1 2.7867(4) 5
Ti1 Te1 2.7867(4) 77

_cod_database_fobs_code 1561866
